# Integration of self-consistent polycrystal plasticity with ... · PDF fileIn this paper, we...

### Transcript of Integration of self-consistent polycrystal plasticity with ... · PDF fileIn this paper, we...

Contents lists available at SciVerse ScienceDirect

Journal of the Mechanics and Physics of Solids

Journal of the Mechanics and Physics of Solids 61 (2013) 2034–2046

0022-50http://d

n CorrNH 038

E-m

journal homepage: www.elsevier.com/locate/jmps

Integration of self-consistent polycrystal plasticitywith dislocation density based hardening laws withinan implicit finite element framework: Application tolow-symmetry metals

Marko Knezevic a,b,n, Rodney J. McCabe a, Ricardo A. Lebensohn a,Carlos N. Tomé a, Cheng Liu a, Manuel L. Lovato a, Bogdan Mihaila a

a Materials Science and Technology Division, Los Alamos National Laboratory, Los Alamos, NM 87545, USAb Department of Mechanical Engineering, University of New Hampshire, Durham, NH 03824, USA

a r t i c l e i n f o

Article history:Received 22 November 2012Received in revised form19 March 2013Accepted 12 May 2013Available online 6 June 2013

Keywords:UraniumConstitutive modelingFinite element methodTextureEBSD

96/$ - see front matter & 2013 Elsevier Ltd.x.doi.org/10.1016/j.jmps.2013.05.005

esponding author at: Department of Mecha24, USA. Tel.: +505 665 7587; fax: +505 667ail address: [email protected] (M. Kn

a b s t r a c t

We present an implementation of the viscoplastic self-consistent (VPSC) polycrystallinemodel in an implicit finite element (FE) framework, which accounts for a dislocation-based hardening law for multiple slip and twinning modes at the micro-scale grain level.The model is applied to simulate the macro-scale mechanical response of a highlyanisotropic low-symmetry (orthorhombic) crystal structure. In this approach, a finiteelement integration point represents a polycrystalline material point and the meso-scalemechanical response is obtained by the mean-field VPSC homogenization scheme. Wedemonstrate the accuracy of the FE-VPSC model by analyzing the mechanical responseand microstructure evolution of α-uranium samples under simple compression/tensionand four-point bending tests. Predictions of the FE-VPSC simulations compare favorablywith experimental measurements of geometrical changes and microstructure evolution.Specifically, the model captures accurately the tension–compression asymmetry of thematerial associated with twinning, as well as the rigidity of the material response alongthe hard-to-deform crystallographic orientations.

& 2013 Elsevier Ltd. All rights reserved.

1. Introduction

Polycrystal plasticity models such as Taylor-type (Kalidindi et al., 1992; Knezevic et al., 2009; Taylor, 1938; Van Houtteet al., 1999) and self-consistent-type models (Lebensohn and Tomé, 1993; Lebensohn et al., 2007) have been rigorouslyformulated and extensively used to understand and predict the mechanical response and microstructure evolution in metalssubject to finite strains. The degree of sophistication necessary to accurately model a material generally depends on thecrystal structure and the number and types of deformation modes active in the material. In this paper, we use α-uranium(α-U) as a model material system to illustrate the predictive capabilities of this modeling framework for low-symmetrymetals. Uranium is an important metal for energy (e.g. metallic nuclear fuels) and defense applications, and is a challengingmaterial to model because of its pronounced mechanical anisotropy. At room temperature, uranium has a low-symmetry

All rights reserved.

nical Engineering, University of New Hampshire, 33 Academic Way, Kingsbury Hall, W119, Durham,8021.ezevic).

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–2046 2035

crystal structure (orthorhombic), and polycrystal plasticity requires activation of as many as four different slip modes, and atleast two different deformation twinning modes. To complicate matters, the operating slip and twinning modes exhibit lowmultiplicity and widely different activation stresses. Consequently, the plastic response is highly anisotropic with markedtension–compression asymmetry and hardening depends strongly on texture and the interactions between the slip andtwin modes. Recently, we showed that a hardening law explicitly based on dislocation density evolution implementedwithin the VPSC homogenization scheme performs well in capturing the anisotropic strain hardening and texture evolutionin α-U (Knezevic et al., 2012; McCabe et al., 2010). Subsequently, the VPSC model of α-U was extended to account for strain-rate and temperature effects (Knezevic et al., 2013b). Comparison of simulations and experiments in these studies allowedus to infer basic information concerning the various slip and twin mechanisms, their interactions, and their role on strainhardening and texture evolution. It was found that the initial texture plays a significant role in determining the level ofplastic anisotropy, and deformation twinning plays a major role in strain hardening behavior and texture evolution in α-U.Hence, it is evident that the accurate modeling of this complex material system requires a crystal-plasticity theoreticalframework that accounts for microstructure evolution, rather than a continuum approach. These early successes provide theincentive for integrating the VPSC-based material subroutine for uranium into a finite element (FE) framework to facilitatepredicting geometrical changes along with microstructure evolution of α-U components. Such integration is necessary forengineering structural and process modeling applications.

The strategy of embedding the mean-field VPSC model at the meso-scale level in an implicit FE analysis was recentlydiscussed (Segurado et al., 2012). In an implicit nonlinear FE formulation, the material constitutive model provides the stressand tangent stiffness matrix. In our approach, the tangent stiffness matrix (Jacobian) is obtained analytically and allows forfast convergence towards stress equilibrium. The FE Jacobian is a function of the viscoplastic tangent moduli (which hasalready been calculated as part of the nonlinear self-consistent homogenization scheme), the elastic stiffness of theaggregate, and the FE time increment.

In this paper, we combine these recent advances and present an implementation of the VPSC polycrystalline model inimplicit finite elements that accounts for a dislocation density based hardening law necessary to model the highlyanisotropic response of α-U. We demonstrate that the VPSC calculations can be performed in the global FE frame rather thanin the co-rotational frame adopted in the original FE-VPSC implementation (Segurado et al., 2012). The added benefit is thatcrystallographic texture stays in the global frame and thus the field and state variables are not regularly rotated between theglobal and co-rotational frame. Simple compression, simple tension, and simple shear tests on polycrystalline uranium areused to demonstrate the accuracy of the FE-VPSC model in ABAQUS by comparing with the results of the stand-alone VPSCmodel. The α-U FE-VPSC model is subsequently used to simulate the mechanical response and texture evolution of α-Ucylinders in simple compression and beams in four-point bending deformation experiments. A total of two cylinders andfour beams, classified by the alignment of the sample axis with respect to the rolled plate direction and the loading directionwere experimentally deformed. Quantitative comparisons with experimental measurements of strain fields by digital imagecorrelation (DIC) mapping, geometrical changes captured optically, and texture evolution by electron backscattereddiffraction (EBSD) based orientation imaging are used to demonstrate the predictive capabilities of the model. We findthat the FE-VPSC simulations capture well the strain field, shifts of the neutral axis of the beams, changes in the cross-section geometry and texture evolution during deformation.

2. Modeling framework

In this section, we outline the salient aspects of the micro-scale hardening law based on dislocation densities for α-U, theVPSC polycrystal plasticity meso-scale model and its implementation in the macro-scale implicit finite element framework.

2.1. Micro-scale model

Plastic deformation in each grain occurs via the activation of both slip and twin modes. The corresponding slip or twinshear rate, _γs on a system, s, is given by the power-law:

_γs ¼ _γo

����� r′ : ms

τsc

�����1=m

signðr′ : msÞ ð1Þ

where r′ is the Cauchy stress deviator, ms is the Schmid tensor associated with slip or twinning system s, _γso is the referenceslip rate on system s, m is the rate sensitivity parameter, and τsc is the resistance of slip or twinning system s. A rate-sensitivity exponent of 0.1 is taken to be the same for all slip and twinning modes.

Early experiments (Anderson and Bishop, 1962; Daniel et al., 1971; Fisher and McSkimin, 1958; Yoo, 1968) established thefollowing four slip modes (0 1 0)[1 0 0], (0 0 1)[1 0 0], ½f110g⟨110⟩and ½f112g⟨021⟩ to operate in α-U. In addition to slip,early studies (Cahn, 1951, 1953; Crocker, 1965; Daniel et al., 1971) confirmed the presence of several twin modes, the twomost prevalent in wrought α-U being f130g⟨310⟩ and f172g⟨312⟩. Consistent with these experimental findings, we considerall of the above slip and twinning systems as potential systems for accommodating the imposed plastic strain in our model.

The equations underlying the single crystal dislocation density based hardening law implemented within VPSC wereproposed in (Beyerlein and Tomé, 2008) and adopted for α-U in (Knezevic et al., 2012) and are briefly summarized here. τsc of

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–20462036

all slip systems or twin variants within one mode α (or family) in a grain are assumed to exhibit the same resistance andthey depend on the accumulated dislocation densities per slip mode. In the case of slip, ταc is expressed as a sum of a frictionstress, ταo, a forest dislocation interaction stress, ταf or , and a dislocation substructure interaction stress, ταsub, i.e.

ταc ¼ ταo þ ταf or þ ταsub ð2Þ

The evolution of ταf or and ταsub is governed by the evolution of the forest ραf or and substructure ραsub dislocation densities, asdescribed below. The effect of forest dislocation density is given by a traditional Taylor law (Mecking and Kocks, 1981):

ταf or ¼ χbαμαffiffiffiffiffiffiffiffiραf or

q; ð3Þ

where χ¼0.9 is a dislocation interaction parameter. Dislocation dynamics simulations show that the contribution tohardening by dislocations stored within substructure such as cell walls can be accounted for using (Madec et al., 2002)

ταsub ¼ ksubμαbα

ffiffiffiffiffiffiffiffiρsub

plog

1bα ffiffiffiffiffiffiffiffi

ρsubp

!: ð4Þ

Here, ksub¼0.086 is an empirical parameter that recovers the Taylor law for low substructure dislocation densities (Madecet al., 2002).

The evolution of the stored forest density ραf or is governed by competition between the rate of storage and the rate ofdynamic recovery:

∂ραf or∂γα

¼∂ραgen;f or∂γα

−∂ραrem;f or

∂γα¼ kα1

ffiffiffiffiffiffiffiffiραf or

q−kα2ð_ε; TÞραf or ;Δραf or ¼

∂ραf or∂γα

Δγα ;j�� ð5Þ

where kα1 is a rate-insensitive coefficient for dislocation storage by statistical trapping of gliding dislocations by forestobstacles and kα2 is a rate-sensitive coefficient that accounts for dynamic recovery by thermally activated mechanisms. Thelatter coefficient, kα2, is given by (Beyerlein and Tomé, 2008)

kα2kα1

¼ χbα

gα1−

kT

Dαb3ln

_ε

_εo

� �� �: ð6Þ

In Eq. (6), k, _εo, gα, and Dα are the Boltzmann constant, a reference strain rate, an effective activation enthalpy and a dragstress, respectively. Dynamic recovery is often associated with thermal activation of dislocation cross-slip and climb, and theformation of dislocation sub-structures is concomitant with these recovery processes. As a consequence, in the model therate of substructure development is coupled to the rate of recovery of all active dislocations through:

Δρsub ¼∑αqαbα

∂ραrem;f or

∂γαΔγα�� �� ð7Þ

where q is a dislocation recovery rate coefficient defining the fraction of an α-type dislocations that do not annihilate butbecome substructure.

In the case of twinning, τβc accounts for a temperature-independent friction term τβo and a latent hardening term couplingslip and twin systems as:

τβc ¼ τβo þ μβ∑βCαβbβbαραf or : ð8Þ

Here μβ , bβ and Cαβ are the elastic shear modulus on the system, the Burgers vector or shear direction of a given system, andthe latent hardening matrix, respectively. The twin transformation is modeled via the composite grain (CG) model (Proustet al., 2007). In brief, CG consists of identifying the twin systemwith the highest shear-rate among all active twin systems, i.e. the Predominant Twin System (PTS) in each grain, and partitioning the grain into a stack of flat ellipsoids having thecrystallographic orientation of the predominant twin and the matrix, respectively. The short axis of the ellipsoids isperpendicular to the twin plane. As more shear is contributed by the twin, a volume fraction is transferred from the parentto the twin and the ellipsoids representing the twins thicken and the ones representing the parent shrink. Except for thevolume transfer coupling, the twin and the parent ellipsoids are treated as independent inclusions in the model.

2.2. Meso-scale model

In order to obtain the mechanical behavior of polycrystalline α-U, we use a self-consistent model. This class of models isbased on the solution of the problem of an ellipsoidal inclusion embedded in a homogenous effective medium. The inclusionis taken to be an individual grain while the homogenous medium represents the polycrystalline aggregate. A detaileddescription of the VPSC model used in this study can be found elsewhere (e.g. Lebensohn et al., 2007). Here we only reportthe equations necessary to follow the details of the FE implementation of the model.

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–2046 2037

The constitutive relations between the Cauchy stress deviator r′ and the viscoplastic strain-rate _εvp at the single-crystallevel at the special location x are given by:

_εvpðxÞ ¼ ∑Ns

s ¼ 1msðxÞ_γsðxÞ; ð9Þ

where the sum runs over all Ns slip and twin systems and ms is the Schmid tensor associated with the slip or twinningsystem s. A linear relation (an approximation of the actual local nonlinear relation, Eq. (9)) is assumed between _εðrÞvpand r′ðrÞ, i.e.

_εðrÞvp ¼MðrÞ : r′ðrÞ þ _εoðrÞ ð10Þ

where MðrÞand _εoðrÞ are the linearized viscoplastic compliance and back-extrapolated strain-rate of grain r, respectively. Thebehavior of the single crystals can be homogenized assuming a linear relation at the effective medium (polycrystal, px) level:

_εðpxÞvp ¼MðpxÞ : r′ðpxÞ þ _εoðpxÞ ð11Þ

where _εðpxÞvp and r′ðpxÞ are the effective (polycrystal) deviatoric strain-rate and stress tensors, respectively, and MðpxÞ and _εoðpxÞ

are the tangent viscoplastic compliance and back-extrapolated strain-rate of an a priori unknown homogeneous linearmedium that represents the behavior of the polycrystal. The usual procedure to obtain the homogenized response of a linearpolycrystal is the linear self-consistent method. The problem underlying the self-consistent method is that of a single crystalr of moduli MðrÞand _εoðrÞ embedded in an infinite medium of moduli MðpxÞ and _εoðpxÞ, which can be obtained using standardself-consistent analysis. The linearization (Eqs. (10) and (11)) eventually lead to uniform stress and strain rate in theellipsoidal domain of the grain.

The above numerical scheme is used to predict the stress–strain response and the microstructure evolution of thepolycrystalline α-U (crystallographic and morphologic texture and hardening evolution), by applying the viscoplasticdeformation to the polycrystal in incremental steps.

2.3. Macro-scale model

A finite element integration point is considered as a polycrystalline material point whose meso-scale mechanicalresponse is obtained by interrogating the VPSC model described above. As a result, we introduce another level ofhomogenization from the meso-scale to the macro-scale. VPSC is implemented as a User Material Subroutine (UMAT) inABAQUS Standard. The total strain increment Δε is divided into the elastic Δεel and viscoplastic Δεvp parts as:

ΔεðpxÞ ¼ΔεðpxÞel þ ΔεðpxÞvp ¼ C−1 : ΔrðpxÞ þ ΔεðpxÞvp ð12Þ

where C is the elastic stiffness of the polycrystalline material point, Δr is the Cauchy stress increment, and Δεvp ¼ΔεvpðrÞ iscomputed using the VPSC model for each polycrystalline material point. Note that superscript (px) is only used in Eq. (12) toshow the continuity between the VPSC material point and the FE code and is explicitly dropped for simplicity. The elasticstiffness, C, is computed using the elastic self-consistent (ELSC) estimate. Note that an ELSC calculation for the determinationof C is implemented in the VPSC code at the beginning of each deformation increment. Hence, the textural changes are alsoaccounted for in determining the elastic modulus of the polycrystalline material element. The single-crystal elasticconstants used for α-U are (Fisher, 1966; Fisher and McSkimin, 1958): C11 ¼ 214:8 GPa,C22 ¼ 198:6 GPa, C33 ¼ 267:1: GPa,C44 ¼ 124:4 GPa, C55 ¼ 73:4 GPa, C66 ¼ 74:3 GPa, C12 ¼ 46:5 GPa, C13 ¼ 21:8 GPa and C23 ¼ 107:6 GPa.

In an earlier work (Segurado et al., 2012), the VPSC calculations were performed in a local co-rotational frame and thetexture was represented in the same co-rotational frame. In our new implementation, the polycrystalline materialundergoes macroscopic rotation due to the macroscopically imposed spinWapp at every time increment. Therefore, eachsingle crystal comprising the polycrystal undergoes rotation due to Wapp

, in addition to a rotation due to the plastic spinWp

and antisymmetric part of the Eshelby tensor Π (Lebensohn et al., 2007). The macroscopically imposed spin Wapp can becomputed from the increment of the macroscopic rotation ΔRapp as Wapp ¼ N_θ, where N is the antisymmetric tensorexpressed in terms of a dual vector n whose components are obtained from ΔRapp as follows: n1 ¼ΔRapp

32 −ΔRapp23 ,

n2 ¼ΔRapp31 −ΔRapp

13 , n3 ¼ΔRapp21 −ΔRapp

12 and _θ¼ arccosð1=2ðΔRappii −1ÞÞ=Δt. The added benefit of the new implementation is

that field and state variables stay in the global frame and are not regularly rotated between the global and co-rotational.The macro-scale constitutive model is formulated incrementally:

_r¼ C : ð_ε−_εvpÞ ð13ÞIntegrating Eq. (13) from time t to t þ Δt gives:

rΔt ¼ C : ðΔε−ΔεvpÞ ð14ÞAt the macroscopic level, the applied load is divided into increments, and the equilibrium at each increment is obtained by

means of the FE analysis in an iterative fashion using a global nonlinear solver with the load increment controlled by time.Once the problem has been solved at time t, the solution for the next time increment requires the polycrystal model to providea tangent stiffness (Jacobian) matrix Ctg ¼ ∂Δr=∂Δε for each material point in order for the FE scheme to compute an initialguess for the nodal displacements at t+Δt. The strain increments obtained from that prediction at each material point, ΔεFE ,

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–20462038

together with the stress rt and the set of internal state variables corresponding to the previous increment are used insideUMAT to calculate a new guess for the stress and the Jacobian at t+Δt. When convergence in stress equilibrium is achieved bythe global nonlinear scheme, the new values (at t+Δt) of the stresses, the internal variables, and the Jacobian matrix areaccepted for every node, and the calculation advances to the next increment.

For a given ΔεFE , the VPSC-based UMAT is based on the minimization procedure described in (Segurado et al., 2012) andis summarized here. The elastic constitutive relation for the stress in the material point at t+Δt is given by:

rtþΔt ¼ rt þ C : Δεel ¼ rt þ C : ðΔε−ΔεvpÞ: ð15Þ

Using Eq. (15) and the viscoplastic constitutive relation, we obtain:

Δε¼ C−1 : Δsþ Δt _εðpxÞvp ðrt þ ΔrÞ ð16Þ

For a given trial strain increment, ΔεFE , we define the residual XðΔrÞ at each material point as a nonlinear function of thestress increment Δr¼ rtþΔt−rt:

XðΔrÞ ¼Δε−ΔεFE ¼ C−1 : Δrþ Δt_εðpxÞvp ðrt þ ΔrÞ−ΔεFE ð17Þ

The condition XðΔrÞ ¼ 0 (i.e. Δε¼ΔεFE) is enforced using a Newton–Raphson (NR) scheme to solve the nonlinear systemof equations. The corresponding Jacobian JNR is given by:

∂XðΔrÞ∂ðΔrÞ ¼ JNRðΔrÞ ¼ Ctg ¼ C−1 þ Δt

∂_εðpxÞvp

∂ðΔrÞ ðrt þ Δr; βti Þ ¼ C−1 þ ΔtMðpxÞðrt þ ΔrÞ ð18Þ

Hence, given a guess Δrk−1 for the stress increment, the new guess is obtained as:

Δrk ¼Δrk−1−J−1NRðΔrk−1Þ : XðΔrk−1Þ ð19Þ

In our formulation, the internal state variables such as crystallographic orientations, axis of the ellipsoids representinggrain, orientation of these ellipsoids etc., βti , are assumed explicit. The approach provides a closed expression for the FEJacobian as a function of the viscoplastic tangent moduli (calculated as part of the VPSC algorithm), the elastic stiffness ofthe aggregate, and the FE time increment. The use of this expression greatly reduces the overall computational cost becausethe stress of the polycrystal and the elasto-viscoplastic tangent stiffness tensor are obtained from the same calculation loop.Moreover, the FE Jacobian allows for the quadratic convergence of the macroscopic nonlinear equations.

3. Applications of the FE-VPSC UMAT for low-symmetry metals

In the following we present several applications used to test the accuracy of the FE-VPSC model in ABAQUS. First, wecompare directly the stress–strain response and texture predicted by the FE-VPSC model against the results obtained usingthe stand-alone SA-VPSC model. Next, we compare the predicted geometrical changes and texture evolution during simplecompression and four-point beam bending with those measured experimentally. In all of the FE-VPSC simulations thatfollow, we use 3D finite elements. Finally, we discuss the effect of texture-induced anisotropy on material flow.

The material used here is straight-rolled polycrystalline α-uranium in its annealed condition. The processing route wasdescribed earlier (Knezevic et al., 2012). The microstructure and texture of the material before testing are shown in Fig. 1.The material has equiaxed twin-free grains with an average grain size of approximately 15 mm. The initial texture shown inFig. 1 was measured by EBSD on a large area of several square millimeters to be representative of the material. Theprocessing route of the starting material induced an orthotropic texture, which allows us to show only one quarter of thepole figures. The pole figures reveal that the material has a strong (001) texture component in the through-thickness (TT3)direction, tilted towards the in-plane 2 (IP2) direction. The (010) and (100) components tend to concentrate away from the(TT3) direction with the peak intensity for (010) being in the in-plane 1 (IP1) direction and the peak intensity for (100) beingin the in-plane 2 (IP2) direction. The measured texture is reduced to 1000 orientations chosen such as to reproduce theexperimental textures shown in Fig. 1. The pole figures of the texture used as input in the simulations are essentiallyindistinguishable from the experimental ones depicted in Fig. 1, and are not shown. Fig. 1 also shows the true-stress true-strain response of the α-U plate along the main rolling directions in simple compression and simple tension. Anisotropy andasymmetry of the mechanical response should be noted. The concave shape of the IPC1 and IPT2 curves is an indication ofdeformation twinning-dominated deformation. We observed in the earlier work (Knezevic et al., 2012) that twins in α-Ugrow rapidly inducing large texture hardening by re-orienting grain from a softer to a harder orientation while the Hall-Petch type hardening (due to grain subdivision) was minimal. For the comparison purpose, it is known that magnesiumalloys exhibit a rapid growth of tensile twins resulting in large texture hardening (Knezevic et al., 2010). The TTC3, IPC2 andIPT1 curves show a classical decreasing hardening rate throughout, which is a sign that the plastic deformation is dominatedby slip. The VPSC constitutive parameters for the material were calibrated in the previous study on the same material(Knezevic et al., 2012 see Tables 2 and 3) and are used in this study.

001 010 100IP2

IP1

Fig. 1. Pole figures and EBSD orientation map showing initial microstructure and texture in the as-annealed straight-rolled uranium. The colors in the mapindicate the crystal direction parallel to the IP1 direction (unit triangle at the bottom). In the corner of the map we illustrate the inverse pole figure for theIP1 direction. The IPF triangle has the crystal reference frame defined as [1 0 0] bottom right, [0 1 0] top left, and [0 0 1] bottom left. Stress-strain responsein compression (C) and tension (T) at room temperature is shown along the directions indicated in the plot of annealed α-uranium. (For interpretation ofthe references to color in this figure caption, the reader is referred to the web version of this article.)

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–2046 2039

3.1. Validation of FE-VPSC with SA-VPSC

For the purpose of validation, we compare the results of the FE-VPSC UMAT implementation against those of the SA-VPSCmodel with simple boundary conditions, i.e. the type of imposed boundary conditions the SA-VPSC model can handle.Simple tension and simple compression up to a strain of 0.2 are simulated using SA-VPSC by imposing 0.002 strainincrements along the corresponding direction, while enforcing zero average stress along the two lateral directions of thesample. The same tests were simulated with the FE-VPSC UMAT and compared with the SA-VPSC model results.We constructed the simple FE models of single linear element C3D8 (8 nodes, and 8 integration points) with displacementsimposed along the 2-direction for compression and tension and stress-free boundary conditions on the lateral faces.In addition, simple shear tests were performed by SA-VPSC as well as FE-VPSC where the same one element model wasused. We applied deformation gradient of F¼ Iþ γ e2⊗e3, with γ ¼ 0:2. This analysis was performed in order to check thecorrect treatment of rotations under finite-deformation kinematics. The predicted stress–strain curves and pole figurespredicted by the two models are in excellent agreement (see Fig. 2). Observe that SA-VPSC does not produce the elasticresponse, which causes some difference with FE-VPSC.

3.2. Compression of α-uranium

Simple compression experiments were performed on cylinders machined from the straight-rolled α-U plate in twodifferent directions, the rolling direction (IPC1) and the through-thickness direction (TTC3). These tests were also used tovalidate the implemented FE-VPSC UMAT and illustrate the effect of texture-induced anisotropy on the mechanical responseof α-U. The FE model consisted of approximately 1000C3D8 elements with the same 1000 grains at each integration point(see Fig. 1). The geometrical changes of the samples compressed to a strain of 0.2 are shown in Fig. 3. Here, the symbolsoverlaid onto the photographs of the deformed cross sections denote the external nodal coordinates of the deformed FEmodel predictions. Note that the TTC3 compressed cylinder preserves a near uniform cross-section and the IPC1 compressedcylinder developed an oval cross-section. The accuracy of our simulation results relative to the geometrical changesmeasured experimentally, demonstrate that the FE-VPSC UMAT implementation accurately predicts the complex deforma-tion behavior (i.e. texture-induced anisotropic material flow) exhibited by α-U. The measured and simulated horizontal andvertical strains are in excellent agreement and are about 0.092 and 0.084 for the cylinder compressed in the direction 3 and0.074 and 0.110 for the cylinder compressed in the direction 1. Computational time associated with a uniaxial deformationsimulation involving 1000 elements containing 1000 grains up to a strain of 0.2 is about 60 h on a regular PC. However ourimplementation can run in parallel and a multiple CPU hardware can substantially reduce the time involved.

3.3. Bending of α-uranium

A detailed evaluation of the FE-VPSC model is presented by comparing the model predictions with the experimentalmeasurements of dimensional changes and microstructure evolution during the four-point bending of α-U beams. Four-point beam bending tests present more stringent tests of the model, as one produces a continuous gradient of strain, fromcompressive conditions in the upper portion to tensile conditions in the bottom portion of the beams. These conditionswere selected for validation of the FE-VPSC models capabilities to predict the effects of the directionality of twinning.

IP2

IP1

001 010 100

IP2

IP1

IP2

IP1

Fig. 2. Predictions of the FE-VPSC UMAT described here compared with the corresponding predictions of SA-VPSC for (a) in-plane compression in2 direction (IPC2), (b) in-plane tension in 2 direction (IPT2) and (c) simple shear in 23 direction of α-uranium: stress–strain curves and pole figures at strainof 0.2 (SA-VPSC top row and FE-VPSC bottom row). The intensity of the contour lines corresponds to 0.7/1.0/1.4/2.0/2.8/4.0/5.7 (see Fig. 1 for colors).

Fig. 3. Comparison of the predictions using the FE-VPSC UMAT and experimentally measured cross-sections of cylinders compressed up to a strain of 0.2 inthe direction 3 (on the left) and in the direction 1 (on the right). The external nodal coordinates of the deformed FEM model are superimposed on theexperimentally deformed samples of uranium.

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–20462040

Depending on the loading direction with respect with to the texture in the beams, we expect to find qualitative differencesbetween the response of the upper (top/compressive) and lower (bottom/tensile) portions of the beam and a shift of theneutral axis. We also provide insights into deformation behavior of α-U during bending.

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–2046 2041

The photograph of the four-point beam testing jig with the test specimen is shown in Fig. 4. We followed the sameexperimental setup as in our earlier work involving titanium (Knezevic et al., 2013a; Nixon et al., 2010). It consisted of a pairof internal pins, moving downwards from the top of the beam, and a pair of external pins, fixed underneath the beam. Theinternal and external pairs of pins were set at center-to-center distances of 76.35 mm and 719.05 mm, respectively. Thetotal displacement of the upper pins was −3.5 mm, corresponding to an axial (longitudinal) strain of the most external fiberof approximately 0.1. The deformed specimens were cut at the midpoint and the final deformed cross-sectionsphotographed. The photographed cross-sections are used to test the accuracy of the FE-VPSC model. Four specimensmachined from the orthotropic plate of α-U were tested along different loading orientations. Specifically, two samples hadthe beam axis aligned with the plate IP1, while the other two samples had the beam axis aligned with the plate IP2. For eachof these two sets of specimens, one sample was loaded in the TT3 direction while the other sample was loaded in the otherin-plane direction normal to the beam axis. As a result, the beams had different starting textures relative to the bendingplane. Our aim is to illustrate the ability of the FE-VPSC model to capture the strong effect of texture-induced anisotropy andasymmetry on the geometrical changes during bending of α-U. The four test configurations are shown in Fig. 5. We show theexperimentally deformed beams, together with the model results. The predicted axial strain distributions are shown. Eachbeam had a square cross-section of 6.35 mm�6.35 mm and a length of 50.8 mm.

Due to the presence of orthotropic symmetry, we only model a quarter of the beam using a structured mesh of 20�5�3elements along the half-length, thickness and half-width, respectively by imposing symmetry boundary conditions. Thedisplacement of the upper pins was modeled by imposing displacement corresponding to experimental values along theloading direction to the upper nodes, located at 6.35 mm from the midpoint. The lower nodes, located at 19.05 mm from themidpoint are constrained along the loading direction (no displacement is allowed along the loading direction) to representthe fixed pins.

After performing a mesh-sensitivity study, we observed that further refinement of the mesh leaves the resultsunchanged and adding more elements only increased the computational time involved. We found that the quadraticelements with reduced integration (C3D20R) provided the best compromise between accuracy of the simulations and thecomputational time involved. These elements were flexible to bend owing to the large number of degrees of freedom(20 nodes) and efficient owing to the reduced number of integration points where the computationally intensivepolycrystalline response is obtained.

Fig. 4. Four-point beam testing jig with a test specimen.

Fig. 5. Test configurations of the four-point beam bending specimens with a sprayed speckle pattern for DIC measurements (left) and corresponding FEmodels showing the axial strain distributions (right). The long axis of the specimens and the loading direction align with the directions of the α-U plate,as follows: 1¼ IP1, 2¼ IP2 and 3¼TT3.

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–20462042

In Fig. 6 we illustrate the comparison between the predicted and measured cross sections of the α-U beams in the finaldeformed state. Here, the symbols overlaid onto the photographs of the deformed cross sections denote the external nodalcoordinates of the deformed FE model predictions and show that the FE-VPSC model accurately predicts the dimensionalchanges of the cross sections for all cases considered here. The model predicts the deviation of the final cross section fromthe initial square shape of the cross section of the beam. This deviation depends on the corresponding beam configurationand deformation direction and reflects the anisotropic character of the mechanical response in α-U induced by the strongeffect of texture. Note that when the through-thickness direction (TT) is perpendicular to the loading direction, the cross-sections of the beams retain an almost square shape, because it is difficult to deform the material along the ⟨001⟩ direction.In turn, the samples deformed in-plane developed wedge-shape cross sections, with more lateral strain when the IP1 of theplate is horizontal. This is consistent with the uniaxial tests results shown in Fig. 1, which show that the IP1 direction issofter than the IP2 direction of the α-U plate. The results also emphasize the importance of the anisotropy of themacroscopic plastic Poisson strain. When a compressive or tensile deformation in a grain result in twinning, the resultingPoisson strain is in a direction perpendicular to ⟨001⟩ because of the crystallography of the twins. When the beams areloaded parallel with TT3, the resulting Poisson strain anisotropy largely occurs in the horizontal cross-section directionresulting in the changes in shape. Below, we explain this in more detail.

As indicated in Fig. 5, speckle patterns were sprayed on one side of each beam and local strain measurements wereobtained using the digital image correlation (DIC) technique (Rastogi et al., 2000). The experimentally measured andpredicted strain fields in the final deformed beams are illustrated in Fig. 7, together with the corresponding experimental

Fig. 6. Comparison of the predicted and measured cross-sections of the α-uranium beams. The external nodal coordinates of the deformed FEM models aresuperimposed on the photographed experimentally deformed beams.

Fig. 7. Comparison of the axial strain contours and the axial strains along the height of the beams simulated with the FE-VPSC against DIC data. Note theshift in the neutral axis of the beams. The lines are the geometric center lines and the dotted curves are the neutral axis lines.

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–2046 2043

and calculated height dependence of the axial strains at the center of the beams. There is a downward shift of the neutralaxis when the beam axis is aligned with the RD direction of the plate, which is a consequence of the material being harder intension than in compression. Likewise there is an upward shift of the neutral axis when the beam axis is aligned with the TD

1-beam axis, 3-loading direction

Top

Middle

Measured

001 010 100IP2

IP1

Predicted

Bottom

Top

Middle

Bottom

2-beam axis, 3-loading direction

2-beam axis, 1-loading direction

Top

Middle

Bottom

1-beam axis, 2-loading direction

Top

Middle

Bottom

Fig. 8. Pole figures showing measured (on the left) and predicted (on the right) texture at the top, middle, and bottom locations for each α-uranium beamat the end of the bending deformation. Arrow indicates the change in the (010) texture component due to twinning as a function of beam height. Theintensity of the contour lines corresponds to 0.7/1.0/1.4/2.0/2.8/4.0/5.7 (see Fig. 1 for colors).

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–20462044

direction of the plate, due to the material being softer in tension than in compression. Again, the agreement of the FE-VPSCmodel predictions and the experimental observations is excellent in all four cases considered here.

Fig. 8 shows the measured and predicted texture evolution of the material. We find that when the beam axis is alignedwith the plate IP1 direction, the (010) peak intensity becomes stronger in the IP2 direction (and weaker in the IP1 direction)

1-beam axis, 3-loading direction 1-beam axis, 2-loading direction

2-beam axis, 3-loading direction 2-beam axis, 1-loading direction

Top

Middle

Bottom

Top

Middle

Bottom

Fig. 9. Inverse pole figure (IPF) maps showing microstructure evolution in the α-uranium beams at the top, middle, and bottom locations for each beam atthe end of the bending deformation. The middle images were taken at the geometric centers of the beams and the top and bottom were 73 mm from thegeometric centers. The colors in these maps indicate the direction of the beam axis with respect to the crystal reference frame. The IPF texture plots in theupper right corner of each image indicate intensities in the IP1 direction. (For interpretation of the references to color in this figure caption, the reader isreferred to the web version of this article.)

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–2046 2045

due to twinning in the top compressive portion of the beam (see the IPC1 stress–strain response in Fig. 1). Likewise, whenthe beam axis is aligned with the IP2, the (010) peak intensity becomes stronger in the IP1 direction (and weaker in the IP2direction) due to twinning in the bottom portion of the beam experiencing a tensile stress state (see the IPT2 stress–strainresponse in Fig. 1). These trends in texture change due to twinning are indicated in the Fig. 8 by a line with an arrow. In themiddle of the beam there is very little texture change, and the texture is expected to be the same as the initial texture.However, due to a small size of EBSD scans taken to measure texture along the height of the beams compared to a very largeEBSD scan taken to measure the initial texture in the Fig. 1, the textures in the middle of the beams are not exactly the sameas the one shown in the Fig. 1, but they are very similar. We associate the small difference between the measured and thepredicted textures shown in the Fig. 8 to the smaller size of the EBSD scans that are perhaps not statistically representativeof the texture in the beams. We reiterate that in the simulations we used the initial texture shown in the Fig. 1, obtainedfrom a very large EBSD scan. Qualitatively, the measured and the predicted changes in the textures in the top portion of thebeams and in the bottom portion of the beams relative to the texture in the middle of the beams (if we assume that thetextures in the middle of the beams were not changing) are in excellent agreement. The twinning activity is furtherillustrated in the Fig. 9. The inverse pole figures also show the trend in the texture evolution in the beams as a function ofheight. We observe that the orientation of the twin lamellas varies with the configurations of the beams. When most of thetwins are oriented vertically, the horizontal flaw of the material is possible through thickening/growth of the twins. Most ofthe twins observed in Fig. 9 are f130g⟨310⟩ twins. The twin plane {130} and shear direction ⟨310⟩ are perpendicular to the[0 0 1] direction. For compression, the shear produced by a f130g⟨310⟩ twin results in contraction along the compressiondirection (usually close to a (0 1 0)) and a macroscopic plastic Poisson extension in the direction perpendicular to both thecompression direction and the [0 0 1] direction (usually close to a (1 0 0)). Similarly for compression, the shear produced bya f130g⟨310⟩ twin results extension along the tension direction (usually close to a (1 0 0)) and a Poisson contraction in thedirection perpendicular to both the tension direction and the [0 0 1] direction (usually close to a (0 1 0)). Because of thestrong starting textures, this effect results in an anisotropic Poisson strain effect culminating in the different shapesobserved in Fig. 6, which the model captures well.

Future work will concentrate on extending the hardening law to include effects such as reverse dislocation motion(Kitayama et al., in press) and de-twinning (Proust et al., 2008), which are important to account for by the model to be ableto perform full-scale performance evaluations of uranium components where any kind of non-proportional loading can beexpected and on applications of the modeling framework developed here in microstructure design (Fast et al., 2008;Kalidindi et al., 2009; Knezevic and Kalidindi, in press) and process design (Knezevic et al., 2008; Shaffer et al., 2010) foruranium components.

4. Conclusions

In this paper we discuss the numerical implementation of a recent VPSC polycrystalline model for low-symmetry metalsinto an FE framework. The VPSC model uses a dislocation density based hardening law and is able to predict the highlyanisotropic mechanical response of low-symmetry metals. We showed that the FE-VPSC implementation can be simplifiedby performing calculations in the global frame rather than in the co-rotational frame adopted in the original FE-VPSCimplementation. First, we verified that the FE-VPSC model reproduces the results of the stand-alone SA-VPSC model forsimple compression, simple tension, and simple shear tests on polycrystalline wrought α-uranium (orthorhombic crystalstructure). Then, the FE-VPSC model was used to simulate the dimensional changes and microstructure evolution in simplecompression and four-point bending tests. We showed that the model successfully predicts the deformed shape of thecylinders and the beam cross sections by direct comparison with experiments performed on α-uranium samples. Inaddition, we demonstrated that the strain fields measured experimentally by digital image correlation strain mappingcompare well with the strain fields predicted by the FE-VPSC model in the final deformed beams. Similarly, we find goodagreement between the corresponding experimental and calculated height dependence of the axial strains at the center ofthe beams. Finally, we show a good agreement of the predicted and measured texture evolution as a function of beamheight. Keeping in mind that the VPSC constitutive law was adjusted previously to an independent set of monotonicexperiments, we emphasize that no additional knobs were available in order to affect the material response in the FE-VPSCsimulations, and the results of the simulations should be regarded as predictions in that sense. Therefore, we conclude thatthe FE-VPSC model is able to capture with great accuracy the evolution of anisotropy and tension–compression asymmetryof the material due to microstructure evolution, as well as the rigidity of the material flow along hard-to-deformcrystallographic directions.

Acknowledgements

This work was supported in part by the US Department of Energy under contract number DE-AC52-06NA25396.M. Knezevic gratefully acknowledges the Seaborg Institute for partial financial support under a Post-Doctoral Fellowshipthrough the LANL LDRD Program. The EBSD work was performed in the electron microscopy laboratory (EML) at Los Alamos.The authors acknowledge T. Beard for help with mechanical testing and J. Crapps for help with setting up the FE model.

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 2034–20462046

References

Anderson, R.G., Bishop, J.W. 1962. The effect of neutron irradiation and thermal cycling on permanent deformations in uranium under load. In: Symposiumon uranium and graphite. The Institute of Metals, London, 17–23.

Beyerlein, I.J., Tomé, C.N., 2008. A dislocation-based constitutive law for pure Zr including temperature effects. Int. J. Plasticity 24, 867–895.Cahn, R.W., 1951. Twinning and slip in α-uranium. Acta Crystallogr. 4, 470.Cahn, R.W., 1953. Plastic deformation of alpha-uranium; twinning and slip. Acta Metall. 1 (49–52), 53–70. IN41-IN45.Crocker, A.G., 1965. The crystallography of deformation twinning in alpha-uranium. J. Nucl. Mater. 16, 306–326.Daniel, J.S., Lesage, B., Lacombe, P., 1971. The influence of temperature on slip and twinning in uranium. Acta Metall. 19, 163–173.Fast, T., Knezevic, M., Kalidindi, S.R., 2008. Application of microstructure sensitive design to structural components produced from hexagonal

polycrystalline metals. Comput. Mater. Sci. 43, 374–383.Fisher, E.S., 1966. Temperature dependence of the elastic moduli in alpha uranium single crystals, part IV (298 to 923 K). J. Nucl. Mater. 18, 39–54.Fisher, E.S., McSkimin, H.J., 1958. Adiabatic elastic moduli of single crystal alpha Uranium. J. Appl. Phys. 29, 1473–1484.Kalidindi, S.R., Bronkhorst, C.A., Anand, L., 1992. Crystallographic texture evolution in bulk deformation processing of Fcc metals. J. Mech. Phys. Solids 40,

537–569.Kalidindi, S.R., Knezevic, M., Niezgoda, S., Shaffer, J., 2009. Representation of the orientation distribution function and computation of first-order elastic

properties closures using discrete Fourier transforms. Acta Mater. 57, 3916–3923.Kitayama, K., Tomé, C.N., Rauch, E.F., Gracio, J.J., Barlat, F., A crystallographic dislocation model for describing hardening of polycrystals during strain path

changes. Application to low carbon steels. Int. J. Plast. 54–69, http://dx.doi.org/10.1016/j.ijplas.2012.09.004, in press.Knezevic, M., Al-Harbi, H.F., Kalidindi, S.R., 2009. Crystal plasticity simulations using discrete Fourier transforms. Acta Mater. 57, 1777–1784.Knezevic, M., Capolungo, L., Tomé, C.N., Lebensohn, R.A., Alexander, D.J., Mihaila, B., McCabe, R.J., 2012. Anisotropic stress-strain response and

microstructure evolution of textured α-uranium. Acta Mater. 60, 702–715.Knezevic, M., Kalidindi, S.R., Fast computation of first-order elastic-plastic closures for polycrystalline cubic-orthorhombic microstructures. Comput. Mater.

Sci. 643–648, http://dx.doi.org/10.1016/j.commatsci.2006.08.025, in press.Knezevic, M., Kalidindi, S.R., Mishra, R.K., 2008. Delineation of first-order closures for plastic properties requiring explicit consideration of strain hardening

and crystallographic texture evolution. Int. J. Plasticity 24, 327–342.Knezevic, M., Lebensohn, R.A., Cazacu, O., Revil-Baudard, B., Proust, G.n.l., Vogel, S.C., Nixon, M.E., 2013a. Modeling bending of α-titanium with embedded

polycrystal plasticity in implicit finite elements. Mater. Sci. Eng. A 564, 116–126.Knezevic, M., Levinson, A., Harris, R., Mishra, R.K., Doherty, R.D., Kalidindi, S.R., 2010. Deformation twinning in AZ31: influence on strain hardening and

texture evolution. Acta Mater. 58, 6230–6242.Knezevic, M., McCabe, R.J., Tomé, C.N., Lebensohn, R.A., Chen, S.R., Cady, C.M., Gray III, G.T., Mihaila, B., 2013b. Modeling mechanical response and texture

evolution of α-uranium as a function of strain rate and temperature using polycrystal plasticity. Int. J. Plasticity 43, 70–84.Lebensohn, R.A., Tomé, C.N., 1993. A self-consistent anisotropic approach for the simulation of plastic deformation and texture development of polycrystals:

Application to zirconium alloys. Acta Metall. Mater. 41, 2611–2624.Lebensohn, R.A., Tomé, C.N., Castaneda, P.P., 2007. Self-consistent modelling of the mechanical behaviour of viscoplastic polycrystals incorporating

intragranular field fluctuations. Philos. Mag. 87, 4287–4322.Madec, R., Devincre, B., Kubin, L.P., 2002. From dislocation junctions to forest hardening. Phys. Rev. Lett. 89, 255508.McCabe, R.J., Capolungo, L., Marshall, P.E., Cady, C.M., Tomé, C.N., 2010. Deformation of wrought uranium: experiments and modeling. Acta Mater. 58,

5447–5459.Mecking, H., Kocks, U.F., 1981. Kinetics of flow and strain-hardening. Acta Metall. Mater. 29, 1865–1875.Nixon, M.E., Lebensohn, R.A., Cazacu, O., Liu, C., 2010. Experimental and finite-element analysis of the anisotropic response of high-purity α-titanium in

bending. Acta Mater. 58, 5759–5767.Proust, G., Tomé, C.N., Jain, A., Agnew, S.R., 2008. Modeling the effect of twinning and detwinning during strain-path changes in magnesium alloy AZ31.

Int. J. Plasticity 25, 861–880.Proust, G., Tomé, C.N., Kaschner, G.C., 2007. Modeling texture, twinning and hardening evolution during deformation of hexagonal materials. Acta Mater.

55, 2137–2148.Rastogi, P., Sutton, M., McNeill, S., Helm, J., Chao, Y. 2000. Advances in two-dimensional and three-dimensional computer vision, In: Photomechanics.

Springer, Berlin Heidelberg, 323–372.Segurado, J., Lebensohn, R.A., Llorca, J., Tomé, C.N., 2012. Multiscale modeling of plasticity based on embedding the viscoplastic self-consistent formulation

in implicit finite elements. Int. J. Plasticity 28, 124–140.Shaffer, J.B., Knezevic, M., Kalidindi, S.R., 2010. Building texture evolution networks for deformation processing of polycrystalline fcc metals using spectral

approaches: applications to process design for targeted performance. Int. J. Plasticity 26, 1183–1194.Taylor, G.I., 1938. Plastic strain in metals. J. Inst. Metals 62, 307–324.Van Houtte, P., Delannay, L., Samajdar, I., 1999. Quantitative prediction of cold rolling textures in low-carbon steel by means of the LAMEL model. Textures

Microstruct. 31, 109–149.Yoo, M.H., 1968. Slip modes of alpha uranium. J. Nucl. Mater. 26, 307–318.